Ab initio studies of propene epoxidation on oxidized silver surfaces
L. M. Molina,∗a
M. J. L´opez,a
and J. A. Alonsoa
Received Xth XXXXXXXXXX 20XX, Accepted Xth XXXXXXXXX 20XX First published on the web Xth XXXXXXXXXX 200X
Ab initio density functional simulations have been performed to study the adsorption of propene on partially oxidized silver surfaces and its interaction with surface oxygen. Two different adsorption conformations for propene are studied, with the molecule either intact or forming an Ag-C3H6-O oxymetallacycle (OMC) intermediate. Then, pathways for propene oxide,
acrolein and propanone formation have been studied in detail, providing insight on the selectivity of the surfaces. We find that formation of acrolein must necessarily take place from OMC intermediates, requiring at least two neighbouring reactive surface oxygen anions. This suggests a strong relation between the concentration of surface oxygen and the selectivity of these surfaces.
Propene oxide (C3H6O) represents a very important precursor
in the production of a broad variety of commodity chemicals1. Traditionaly, it has been produced by complex, expensive and environmentaly unfriendly processes, which create many by-products and waste. For this reason, the search for a more di-rect and inexpensive synthesis route has received considerable attention during the last 10 years. In 1998, Haruta and cowork-ers showed that small gold nanoparticles supported on TiO2
form a promising heterogeneous catalyst for the direct epox-idation of propene by an H2/O2gas mixture2. Afterwards, a
lot of effort has been devoted to clarifying the mechanisms of the reaction (active sites, pathways, etc...) in order to im-prove their performance. The ultimate goal is to produce more active catalysts with higher conversion rates and lower hydro-gen consumption. Among the various aspects of the catalysts’ performance that have been analyzed, two of the main ones are the influence of particle size and the type of oxide support on the activity and selectivity3–5. Particles with a size of 2-5 nm seem to provide the best selectivity, although small gold clusters containing only a few atoms have also been found ac-tive for this reaction6. Concerning the type of support, the most active catalysts are found supported on mesoporous ti-tanosilicates7–10; on these systems, a reaction mechanism has been proposed based on hydrogen peroxide (H2O2) synthesis
at the gold nanoparticles, followed by oxidation of propene at Ti sites isolated within the SiO2 network. In the case of
TiO2substrate, the oxide/gold interfacial region seems to play
a very important role, with propene reacting there with surface oxygen atoms to form key oxymetallacycle (OMC)
intermedi-a Departamento de F´ısica Te´orica, Universidad de Valladolid, E-47011
Valladolid, Spain. Fax: (34) 983423013; Tel: (34) 983185062; E-mail: email@example.com
Aside from activity and selectivity, another key issue is the hydrogen consumption. There is an active search for systems where it is only sparingly used or even not necessary for O2
activation to peroxo species. With this purpose, the alternative approach of using clusters or nanoparticles of other noble met-als or alloys is currently being studied14; it is well known that
silver is a very active and widely used catalyst for the epoxi-dation of ethene15–19. However, when trying to use this metal
for epoxidation of larger alkenes, problems arise because of the competitive oxidation of terminal -CH3groups to an
alde-hyde20–22, which makes obtention of a highly selective cata-lyst problematic. This approach has been the focus of recent experiments in the group of S. Vajda, where it has been shown that supported Ag nanoparticles are actually able to directly epoxidize propene from O2, although the aldehyde by-product
(acrolein) is also produced23. Interestingly, the selectivity was found to be highly dependent on the size of the nanoparticles.
The ab initio density functional calculations for the partial oxidation of propylene were carried out using the DACAPO code26, which expands the wavefunctions in a plane-waves basis set27, and uses ultrasoft pseudopotentials28for treating the electron-ion interaction. The PW91 functional29was used for exchange-correlation, and a 30 Ryd cutoff energy was em-ployed for the plane waves expansion of the wave functions. It was tested that such value gives binding energies which are converged within 0.05 eV. The partially oxidized Ag(111) sur-face was modeled using a 4-layer metal slab, with the oxide on the first one. The first two layers are relaxed, while the two layers at the bottom are kept frozen at their bulk positions. The unit cells in the x and y directions are large enough (see discussion below) as to prevent sizable mutual interactions be-tween adsorbed propene molecules in neighbouring unit cells. A(2×2×1)k-point sampling was found to give converged total energies for the unit cells employed. The vacuum separa-tion between slabs was set to 11 ˚A, ensuring binding energies converged within 0.01 eV. It was tested that, for this type of surfaces, dipole corrections were negligible. For each struc-ture, the electronic degrees of freedom were optimized until total energies were converged with a precision of 5·10−5eV. On each reaction stage, the equilibrium structures were found by a BFGS optimization30, until the maximum force on the atoms was below 0.03 eV/ ˚A(ensuring a precision in binding energies better than 0.01 eV).
Energy barriers were calculated by a constrained minimiza-tion method, involving several simulaminimiza-tions where the reacminimiza-tion coordinate (C-O or C-H bond distance) was restricted at in-creasingly smaller values, while allowing the rest of the sys-tem to freely relax31. At distances nearby the transition state,
various possible conformations of the molecule are relaxed under the mentioned bond distance constraints, until a reliable transition state (characterized by a local energy maximum) is found.
Figure 1 shows the relaxed structures for two alternative mod-els of the silver surface oxide32,33, with either Ag1.83O (top)
or Ag2O (bottom) stoichiometry. The motivation for
study-ing such two different situations arises from their qualitatively different character. In the first case (Ag1.83O) there are two
different types of Ag atoms, either non-oxidized (the ones in the center of Ag-O hexagons) or oxidized. Overall, within the considered unit cell (shown in Fig. 1), the oxidized first layer contains 11 silver atoms (9 oxidized, and 2 non-oxidized) and 6 oxygen atoms, giving an overall stoichiometry of Ag11O6,
which we label as Ag1.83O. In the other case (Ag2O) all silver
atoms are oxidized, forming strong bonds with surface oxygen
anions. The depicted unit cell contains 12 silver and 6 oxygen atoms. Choosing such structures for partially oxidized silver is motivated by recent experimental and theoretical studies of this surface. Early Scanning Tunneling Microscopy (STM) studies by the group of D. A. King34,35proposed a Ag1.83O
conformation for the oxidized Ag(111) surface (later on, this model of the surface has been used to perform simulations of ethene epoxidation). More recently, STM experiments by Schmid et al.36 and by Schnadtet al.37, both supported by DFT simulations, suggest that the Ag2O model of the surface
reproduces more accurately the observed features.
Fig. 1Structure of Ag1.83O (upper panel) and Ag2O (bottom panel) surface oxides. The views in the upper part show a large region of the surface, with the rombohedral unit cell highlighted. Large and small circles represent Ag and O atoms, respectively. For clarity, the silver atoms in the oxidized layer are highlighted in color. The views at the lower part show the side section of the four-layers slab employed in the simulations.
propene (C3H6) at either of the surface oxides. The relaxed
structures and binding energies for adsorption of one propene molecule per unit cell are shown in Figure 2. The propene binding energy BE(C3H6) is defined as:
BE(C3H6) =E(C3H6) +E(AgxOy)−E(C3H6/AgxOy) that is, the difference between the sum of the energies of the separate fragments (gas-phase propene and the silver oxide surface) and the total energy of the propene molecule adsorbed on the surface. Negative values therefore represent endother-mic (i.e., unfavourable) binding. We will focus on the two key reaction stages, namely the initial adsorption of propene through interaction between the substrate and the intact dou-ble C=C bond, and the formation of strongly bound oxymet-allacycle (OMC) intermediate compounds. In the latter case, the double C=C bond breaks while two covalent bonds (a C-O bond and a C-Ag bond) are formed with the surface. This type of reaction intermediates have been identified as crucial during the process of formation of epoxides, both in the case of ethene epoxidation on silver catalysts38, as well as in the case of propene epoxidation on gold nanocatalysts6,11. The final stage of either ethene oxide or propene oxide produc-tion then involves the closing of the C-C-O cycle by breaking the O-surface covalent bond and at the same time forming a new C-O bond, followed by desorption of the product from the surface. In the case of propene epoxidation on gold, there is ample evidence that such process takes place right at the gold-oxide interface11
The upper panel in Figure 2 shows various adsorption con-figurations for intact propene and for the oxymetallacycle at the Ag1.83O surface oxide, which is characterized by the
co-existence of unoxidized and oxidized surface Ag atoms. The isomer in (a) represents the most stable configuration, with the C=C bond on top of the unoxidized Ag atom which lies in the middle of the Ag-O-Ag-O honeycomb structure. The adsorp-tion energy is moderate, 0.37 eV, and the C-Ag bond distances are not too short (2.5-2.6 ˚A), indicating that the chemical in-teraction between the double C=C bond and the metal atom is not strong. On the contrary, in configuration (b) the propene C=C bond interacts strongly with an oxidized Ag atom, and the C-Ag bond distances are much shorter, about 2.2 ˚A; how-ever, the binding energy of propene is smaller (0.15 eV). This happens because the total binding energy includes the cost of the surface reconstruction taking place during propene adsorp-tion, which in this case is quite high; the Ag atom is lifted up, while one oxygen atom moves down. As a result, despite of an intrinsically stronger binding of propene with the sur-face Ag atom, such conformation becomes less stable. It must be noted that the structural arrangement in (b), as well as the binding energy, are almost identical to the conformation found by Bocquet and Loffreda for ethene adsorption on the same type of surface silver oxide38.
Fig. 2Some relevant structures and binding energies for C3H6
adsorption at Ag1.83O (upper panel) and Ag2O (lower panel) surface
oxides. See main text for definition of binding energy.
The results for propene adsorption at the Ag2O surface
ox-ide are shown in the lower panel of Figure 2. Conformations (g) and (h) represent adsorption of intact propene on the two unequivalent types of surface Ag atoms, which are both oxi-dized for this type of oxide. In both cases the binding is quite weak (smaller than 0.2 eV), confirming the more reactive char-acter of non-oxidized metal atoms towards the initial adsorp-tion of propene. The formaadsorp-tion energy of the OMC interme-diates is, as it also happened for Ag1.83O, rather small, being
thermoneutral or slightly endothermic (conformations i-k).
Reactivity and selectivity at Ag1.83
We now discuss the reaction pathways for either propene oxide (CH3CHCH2O), propanone (CH3COCH3) or acrolein
(CH2CHCHO) formation at the Ag1.83O surface oxide. To do
this, we will make use of a reasonable assumption: all these products can be formed starting from a common reaction in-termediate, namely the adsorbed oxymetallacycle. The path-way towards propene oxide involves the formation of a cova-lent O-C bond. We will later see that the simulations show that this step takes place together with the breaking of the oxygen-surface bonds. On the other hand, the first step to-wards acrolein production involves the reaction between one of the hydrogen atoms in the methyl group of the adsorbed OMC intermediate and a neighbouring surface oxygen atom. Finally, the formation of either propanal or propanone in-volves hydrogen transfer from one of the carbon atoms in the double C=C bond of propene to the other carbon atom, with simultaneous formation of a double C=O bond.
We start by considering propene adsorbed on oxidized Ag atoms. Figure 3 shows the relative energies (with respect to gas-phase propene) and the corresponding relaxed structures for several key steps of the reaction. It must be noted that, in order to find favourable reaction pathways, two different OMC conformations are considered for either propene oxide or acrolein production. The reason lies in the requirement of a close distance between the propene methyl group and sur-face oxygen atoms. The most stable OMC arrangement in this surface (conformer (c) in Fig. 2), characterized by a 0.22 eV binding energy, has a methyl group far from any surface oxygen, making its dehydrogenation very difficult. Therefore, we have only evaluated, from such conformation, the energy barrier towards propene oxide formation. If we consider the slightly less stable alternative conformation with the OMC bonded to oxygen through the terminal C atom (configuration (d) in Fig. 2), now the situation changes and it becomes feasi-ble for one of the H atoms in the propene methyl group to react with a neighbouring surface oxygen atom. Therefore, we have
Fig. 3Pathways for either acrolein or propene oxide formation at
the Ag1.83O surface oxide. The energy reference (0.0 eV) is taken as
the energy of the gas-phase propene molecule far from the surface (that is, energy values reflect binding energies with reversed sign).
evaluated three possible energy barriers, correponding respec-tively to the propene oxide formation from configurations (c) and (d), and to the propene dehydrogenation from configura-tion (d). In all cases, the barriers are moderate (of the order of 0.6-0.8 eV), suggesting that both propene oxide and acrolein can be produced during the reaction. The relaxed structures as well as the corresponding potential energies for each transition state are shown as insets in Figure 3.
In the case of propene oxide formation, it is interesting to analyze the energy barriers for each of the two OMC confor-mations studied. The barrier for isomer (c) is 0.2 eV higher than the one for isomer (d). We have found that this differ-ence arises solely because of the stability differdiffer-ence between the initial states; the relative energies of the transition states in both cases are nearly the same (+0.54 and +0.56 eV). One can understand this fact by looking at the relaxed transition state (TS) structures, which are almost identical. The transi-tion states are both characterized by a bond distance for the C-O bond being formed of around 2.0 ˚A. On each case, we also find a very weak interaction between the forming propene oxide entity and the surface, with rather large oxygen-surface bond distances. Given the structural similarities, it is no sur-prising to find similar binding energies. We will later see that the weak interaction of the propene oxide transition state with the surface is a general characteristic of this type of oxide sur-faces, as it also occurs for the Ag2O surface.
or acrolein. However, the higher stability of the (c) conforma-tion, which can lead only to propene oxide formaconforma-tion, suggests that the catalyst will be more selective towards propene oxide. As for the structural characteristics of the transition state for acrolein production, we find an O-H distance of 1.6 ˚A, and a C-H distance of 1.18 ˚A. At this point, the C-H bond is quite weakened, but still keeps its integrity. For smaller O-H dis-tances, the C-H bond completely breaks. It must be noted that the process of formation of the O-H bond also takes place to-gether with the breaking of the C-Ag bond between the OMC and the surface; this bond is almost broken for the transition state.
Fig. 4Pathway for propanone formation at the Ag1.83O surface oxide. The OMC is formed at oxidyzed Ag atoms. Same energy conventions as in Figure 3.
We have also considered the formation of propanone (CH3COCH3) starting from the OMC conformation shown
in Fig. 2c. It must be noted that formation of propanal (CH3CH2CHO) is also a feasible process, provided that the
initial OMC conformation has the oxygen atom bonded to the terminal carbon atom (that is, as in the conformation shown in Fig. 2d). However, since this conformer is 0.2 eV less stable than the conformation shown in Fig. 2c, it is clear that the surface will be more selective towards propanone for-mation. Therefore, we have only analyzed the production of propanone. The results for the energy barrier are shown in Figure 4. We obtain a barrier height of 0.75 eV, almost the same as the one for propene oxide formation from the same OMC reaction intermediate. This suggests a comparable se-lectivity of this oxide surface towards both propene oxide and propanone. At the transition state, the hydrogen atom being transferred is located around 1.55 ˚A away from the terminal carbon atom. Interestingly, at the TS the molecule is now still relatively close to the surface, which should result in a sizable interaction with it.
Next, we have studied the reaction pathways involving
ad-Fig. 5Pathway for propene oxide formation at the Ag1.83O surface oxide. The path involves adsorption of propene and formation of OMC at non-oxidyzed Ag atoms. Same energy conventions as in Figure 3.
sorption of propene and OMC formation at non-oxidized Ag atoms. Figure 5 illustrates the pathway for propene oxide pro-duction when propene initially binds at the unoxidized surface Ag atoms. Initial propene adsorption at those sites is slightly stronger than at oxidized Ag atoms. For the formation of propene oxide, the reaction proceeds in two steps, the first one being the formation of the OMC intermediate, and the second the formation of propene oxide. The first step appears to be the most difficult one, since the OMC intermediate is 0.44 eV less stable than adsorbed propene. Due to this feature, the energy barrier necessary to form propene oxide is very low (0.27 eV, around one half of the corresponding barrier for OMC formed at oxidized Ag atoms).
The situation for acrolein formation at non-oxidized Ag atoms is very interesting. The OMC conformation is not fa-vorable towards acrolein production, since the propene methyl group is placed far away from any surface oxygen anion. Therefore, we have analyzed the possibility of hydrogen trans-fer from the methyl group of intact propene adsorbed at an unoxidized Ag atom (that is, the configuration shown on Fig-ure 2a). Such process is not feasible, since the energy rises steadily (by about 0.6 eV) as the hydrogen atom is detached from the -CH3group while forming a surface hydroxyl (-OH)
group. A Transition State is never found, and all along this pathway the forces are driving the hydrogen atom back to propene. This means that we can disregard such process, and therefore conclude that the only possible precursor towards acrolein formation is the OMC conformation.
hy-drogen detaches from the methyl group and the C=C double bond changes its location within propene. In the acrolein path-way shown in Figure 3, which starts from a OMC conforma-tion, hydrogen abstraction becomes easy (although it requires a small activation energy) because a strong C-O covalent bond is already formed. Then, the propene C=C double bond is transformed into a C-C single bond, and it becomes much eas-ier to transfer the hydrogen atom and to form a C=C bond between the methyl group and the central carbon atom. The fi-nal conclusion is that, while unoxidized Ag atoms are reactive towards propene oxide production, the formation of acrolein seems to require a higher degree of oxidation of the Ag sur-face.
Reactivity and selectivity at Ag2
Finally, we have studied the reactivity and selectivity of the alternate model for the partially oxidized Ag surface, with Ag2O stoichiometry. Figure 6 shows the energy diagram for
either propene oxide (upper panel), propanone (middle panel), or acrolein production (lower panel). Overall, the results are qualitatively similar to the ones in Figure 3 (that is, reaction at oxidized Ag atoms). As it was discussed in section III, ad-sorption of propene is weak, and the relative stability of OMC intermediates is small as well. As for the reaction barrier, we find again barriers of 0.5-0.7 eV, indicating the feasibility of the studied reaction pathways at the typical reaction tempera-tures (100-200oC). At this point, it is interesting to compare the structural features of the propene oxide transition state in this case with the analogous situations for the Ag1.83O model
surface. In all cases, the structures of the transition state are re-markably similar, with a C-O bond distance of approximately 2.0 ˚A, and a rather weak interaction with the surface (the bond distance between the oxygen atom within the metallacycle and Ag surface atoms is quite stretched, of about 2.5 ˚A). The di-rect consequence of the weak TS-surface interaction is a rel-atively constant value of the binding energy of the transition state on a variety of situations (namely, the type of oxide sur-face). Such binding energy will be determined alone by the en-ergetic cost (with respect to gas-phase propene oxide, that is, the final state) of breaking one of the C-O bonds (with an equi-librium length of 1.46 ˚A) and expanding it to a bond length of around 2.0 ˚A. Therefore, the size of the reaction energy bar-rier will only depend on the binding energy of the initial state (the OMC intermediate), which actually varies due to both the structural features of the oxide surface and the exact metalla-cycle conformation.
The formation of propanone takes place starting from the most stable OMC intermediate (the same configuration which is also able to transform into propene oxide). The barrier for
Fig. 6Pathways for propene oxide (upper panel), propanone
(middle panel) and acrolein (bottom panel) formation at the Ag2O
surface oxide. Same energy conventions as in Figure 3.
hydrogen transfer from the central to the terminal carbon is 0.77 eV, about 0.1 eV larger than the barrier for propene oxide formation. Therefore, in this case the surface will be slightly more selective towards propene oxide formation. Again, the possible formation of propanal starting from the OMC con-figuration in Fig. 2j cannot be ruled out, although it is quite probable that the energy barrier will be higher that the one found for acrolein formation (the corresponding competitive process).
starting configuration, with the propene CH3group close to a
surface oxygen anion, an OMC configuration higher in energy than the global minimum (precisely by around 0.2 eV) must be considered. This leads to a decrease of the reaction barrier, although the relative stability of the transition states for both propene oxide and acrolein formation are actually the same. The final conclusion is that both types of products are likely to form, probably with similar selectivity towards them.
In this paper, we have studied the adsorption of propene at two types of oxidized silver surfaces, as well as the possible routes for either its epoxidation or acrolein formation, by re-action with surface oxygen anions. We have also studied for-mation of propanone. Several important conclusions can be drawn from the results of the ab initio simulations. First of all, propene seems to adsorb preferentially at unoxidized Ag atoms (assuming that they exist on the surface), meaning that a situation where the catalyst is only partially oxidized will enhance its reactivity. In all cases, the reaction energy bar-rier for the rate-limiting step (desorption of OMC metallacycle into propene oxide by closing of the C-O-C cycle) lies in the range 0.5-1.0 eV, suggesting that the epoxidation reaction can take place at moderate temperatures. Formation of acrolein can also take place with moderate energy barriers, very simi-lar to the ones calculated for propene oxide production. As for the reaction mechanisms, we have found that acrolein forma-tion must necessarily take place from an OMC intermediate. This means that at least two oxygen adatoms must be close to each other on the surface during formation of acrolein, one of them being part of the OMC intermediate, and another one be-ing able to react with the propene methyl group by transfer of one hydrogen atom. This again gives support to the idea of a higher selectivity of partially-oxidized silver surfaces towards propene oxide production.
Considering the case of a partially oxidized silver nanopar-ticle, where oxygen is expected to concentrate at the most reactive sites (normally low-coordination ones, as edges and corners), the results obtained for extended surfaces suggest that the selectivity will show sizable changes from one type of site to the other. Furthermore, as the relative concentra-tion of highly reactive sites around a nanoparticle depends on its size, a noticeable change in selectivity can be expected for silver nanoparticles of varying size.
Finally, let us mention that propanone can also be formed on this type of system, since the calculated energy barriers are very similar to the ones for propene oxide formation. Neither can we rule out a significant production of propanal; however, a smaller intrinsic stability of the OMC initial state makes propanone formation more probable.
Work supported by the Spanish MICINN and the Eu-ropean Development Fund (grants MAT2008-06483-C03-01 and MAT 2011-22781) and by Junta de Castilla y Leon (grant VA158A11-2). We acknowledge the suport of the spanish su-percomputing network (RES) by the computing time allocated at the BSC (Barcelona) and Altamira (University of Cantabria) nodes.
1 T. A. Nijhuis, M. Makkee, J. A. Moulijn and B.M.Weckhuysen,Ind. Eng. Chem. Res., 2006,45, 3447.
2 T. Hayashi, K. Tanaka and M. Haruta,J. Catal., 1998,178, 566. 3 M. Haruta,CATTECH, 2002,6102.
4 J. Huang and M. Haruta,Res. Chem. Intermed.2012,38, 1.
5 C. X. Qi, J. H. Huang, S. Q. Bao, H. J. Su, T. Akita and M. Haruta,J. Catal., 2011,281, 12.
6 S. Lee, L. M. Molina, M. J. Lopez, J. A. Alonso, B. Hammer, B. Lee, S. Seifert, R. E. Winans, J. W. Elam, M. J. Pellin and S. Vajda,Angew. Chem. Int. Ed., 2009,48, 1467.
7 L. Cumaranatunge and W. N. Delgass,J. Catal., 2005,232, 38. 8 J. Huang, T. Takei, T. Akita, H. Ohashi and M. Haruta,Appl. Catal. B,
9 J. Lu, X. Zhang, J.J. Bravo-Su´arez, T. Fujitani and S.T. Oyama,Catal. Today, 2009,147, 186.
10 B. Taylor, J. Lauterbach and W. N. Delgass,Catal. Today, 2007,123, 50. 11 T. A. R. Nijhuis, T. Visser and B. M. Weckhuysen,Angew. Chem. Int.
Ed., 2005,44, 1115.
12 D. Torres, N. Lopez, F. Illas and R. M. Lambert,Angew. Chem. Int. Ed., 2007,46, 2055.
13 A. Roldan, D. Torres, J. M. Ricart and F. Illas,J. Mol. Catal A, 2009,
14 F. R. Negreiros, E. Apra, G. Barcaro, L. Sementa, S. Vajda and A. For-tunelli,Nanoscale, 2012,4, 1208.
15 A. Kokalj, A. dal Corso, S. de Gironcoli and S. Baroni,Surf. Sci., 2003,
16 A. Kokalj, A. dal Corso, S. de Gironcoli, S. Baroni, Surf. Sci., 2004,
17 A. Kokalj, P. Gava, S. de Gironcoli and S. Baroni,J. Phys. Chem. C, 2008,112, 1019.
18 S. Linic and M. A. Barteau,J. Am. Chem. Soc., 2003,125, 4034. 19 M. -L. Bocquet, A. Michaelides, D. Loffreda, P. Sautet, A. Alavi and D.
A. King,J. Am. Chem. Soc., 2003,125, 5620.
20 J. R. Monnier and G. W. Hartley,J. Catal., 2001,203, 253.
21 X. Liu, R. J. Madix and C. M. Friend,Chem. Soc. Rev., 2008,37, 2243. 22 S. Hawker, C. Mukoid, J. P. S. Badyal and R. M. Lambert,Studies in
Surf. Sci. and Catal., 1990,55, 739.
23 L. M. Molina, S. Lee, K. Sell, G. Barcaro, A. Fortunelli, B. Lee, S. Seifert, R. E. Winans, J. W. Elam, M. J. Pellin, I. Barke, V. von Oeyn-hausen, Y. Lei, R. J. Meyer, J. A. Alonso, A. F. Rodriguez, A. Kleibert, S. Giorgio, C. R. Henry, K. H. Meiwes-Broer and S. Vajda,Catal. Today, 2011,160, 116.
24 A. Klust and R. J. Madix,J. Am. Chem. Soc., 2006,128, 1034. 25 W. Huang, Z. Jiang and J. M. White,Catal. Today, 2008,131, 360. 26 See DACAPO web page at Danish Technical University:
27 M.C. Payne, M. P. Teter, D. C. Allan, T. A. Arias and J. D. Joannopoulos,
Rev. Mod. Phys., 1992,64, 1045.
29 J. P. Perdew, J. A. Chevary, S. H. Vosko, K. A. Jackson, M. R. Pederson, D. J. Singh and C. Fiolhais,Phys. Rev. B, 1992,46, 6671.
30 D. C. Liu and J. Nocedal,Math. Program., 1989,45, 503.
31 A. Alavi, P. Hu, T. Deutsch, P. L. Silvestrelli and J. Hutter,Phys. Rev. Lett., 1998,80, 3650.
32 W.-X. Li, C. Stampfl and M. Scheffler,Phys. Rev. Lett., 2003,90, 256102. 33 C. I. Carlisle, D. A. King, M. -L. Bocquet, J. Cerda and P. Sautet,Phys.
Rev. Lett., 2000,84, 3899.
34 A. Michaelides, M. -L. Bocquet, P. Sautet, A. Alavi and D. A. King,
Chem. Phys. Lett., 2003,367, 344.
35 M. -L. Bocquet, A. Michaelides, P. Sautet and D. A. King,Phys. Rev. B, 2003,68, 075413.
36 M. Schmid, A. Reicho, A. Stierle, I. Costina, J. Klikovits, P. Kostelnik, O. Dubay, G. Kresse, J. Gustafson, E. Lundgren, J. N. Andersen, H. Dosch and P. Varga,Phys. Rev. Lett., 2006,96, 146102.
37 J. Schnadt, A. Michaelides, J. Knudsen, R. T. Vang, K. Reuter, E. Laegs-gaard, M. Scheffler and F. Besenbacher, Phys. Rev. Lett., 2006, 96, 146101.